#------------------------------------------------------------------------------
#$Date: 2016-02-19 16:29:56 +0200 (Fri, 19 Feb 2016) $
#$Revision: 176759 $
#$URL: svn://www.crystallography.net/cod/cif/2/00/82/2008227.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2008227
loop_
_publ_author_name
'Millet, Patrice'
'Henry, Jean-Yves'
'Galy, Jean'
_publ_section_title
;
 The vanadium oxide bronze η-NaₓV₂O₅ (x = 1.286)
;
_journal_issue                   3
_journal_name_full               'Acta Crystallographica Section C'
_journal_page_first              276
_journal_page_last               279
_journal_paper_doi               10.1107/S010827019801587X
_journal_volume                  55
_journal_year                    1999
_chemical_formula_iupac          'Na4.5 V7 O17.5'
_chemical_formula_structural     'Na4.5 O17.5 V7'
_chemical_formula_sum            'Na4.5 O17.5 V7'
_chemical_formula_weight         740.03
_chemical_name_systematic        ' sodium vanadate'
_space_group_IT_number           13
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yc'
_symmetry_space_group_name_H-M   'P 1 2/c 1'
_cell_angle_alpha                90.
_cell_angle_beta                 109.07(3)
_cell_angle_gamma                90.
_cell_formula_units_Z            4
_cell_length_a                   15.181(9)
_cell_length_b                   5.0319(8)
_cell_length_c                   20.760(4)
_cell_measurement_reflns_used    25
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      26.07
_cell_measurement_theta_min      2.82
_cell_volume                     1498.8(10)
_computing_cell_refinement       'CAD-4 EXPRESS'
_computing_data_collection       'CAD-4 EXPRESS (Enraf-Nonius, 1993)'
_computing_data_reduction        'CRYSTALS (Watkin et al., 1985)'
_computing_molecular_graphics    'ORTEPIII (Burnett & Johnson, 1996)'
_computing_publication_material  SHELXL97
_computing_structure_refinement  'SHELXL97 (Sheldrick, 1997)'
_computing_structure_solution    'SIR92 (Altomare et al., 1994)'
_diffrn_ambient_temperature      293(2)
_diffrn_measurement_device       'Enraf-Nonius CAD-4'
_diffrn_measurement_method       ω-2θ
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.046
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -21
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       28
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            4983
_diffrn_reflns_theta_max         30
_diffrn_reflns_theta_min         1
_diffrn_standards_decay_%        0.2
_diffrn_standards_interval_count 250
_diffrn_standards_interval_time  60
_diffrn_standards_number         6
_exptl_absorpt_coefficient_mu    4.401
_exptl_absorpt_correction_T_max  0.802
_exptl_absorpt_correction_T_min  0.554
_exptl_absorpt_correction_type   '\y scan (North et al., 1968)'
_exptl_crystal_colour            'metallic dark blue'
_exptl_crystal_density_diffrn    3.280
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'platelet '
_exptl_crystal_F_000             1402
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.05
_refine_diff_density_max         '1.471 e \%A^-3^ at 0.79\%A from V2'
_refine_diff_density_min         '-1.301 e \%A^-3^ at 0.72\%A from V3'
_refine_ls_extinction_coef       4E-5(14)
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_all   0.963
_refine_ls_goodness_of_fit_obs   1.176
_refine_ls_number_parameters     264
_refine_ls_number_reflns         4983
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.963
_refine_ls_restrained_S_obs      1.176
_refine_ls_R_factor_all          0.106
_refine_ls_R_factor_obs          0.045
_refine_ls_shift/esd_max         0.001
_refine_ls_shift/esd_mean        0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w = 1/[σ²(Fo²)+(0.0664P)²] where P = (Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.127
_refine_ls_wR_factor_obs         0.112
_reflns_number_observed          2388
_reflns_number_total             4354
_reflns_observed_criterion       I>2\s(I)
_cod_data_source_file            br1224.cif
_cod_data_source_block           br1224
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 

The following automatic conversions were performed:

'_refine_ls_weighting_scheme' value 'calc w =
1/[\s^2^(Fo^2^)+(0.0664P)^2^] where P = (Fo^2^+2Fc^2^)/3' was changed
to 'calc'. New tag '_refine_ls_weighting_details' was created. The
value of the new tag was set to 'w = 1/[\s^2^(Fo^2^)+(0.0664P)^2^]
where P = (Fo^2^+2Fc^2^)/3'.

Automatic conversion script
Id: cif_fix_values 3143 2015-03-26 13:38:13Z robertas 
;
_cod_original_cell_volume        1498.80(10)
_cod_original_sg_symbol_H-M      'P 2/c'
_cod_database_code               2008227
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_thermal_displace_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_disorder_group
_atom_site_type_symbol
V1 0.14470(6) 0.91921(18) 0.81807(4) 0.00711(19) Uani d . 1 . V
V2 0.40299(6) 0.85641(17) 0.76864(4) 0.00720(18) Uani d . 1 . V
V3 0.48782(6) 0.90070(19) 0.56437(4) 0.00702(19) Uani d . 1 . V
V4 0.06343(6) 0.9129(2) 0.65012(4) 0.0073(2) Uani d . 1 . V
V5 0.69879(6) 0.8988(2) 0.52283(4) 0.00725(19) Uani d . 1 . V
V6 0.27552(6) 0.90049(19) 0.60617(4) 0.00723(19) Uani d . 1 . V
V7 0.90714(6) 0.8832(2) 0.47782(4) 0.0091(2) Uani d . 1 . V
Na1 0.0000 0.3997(7) 0.7500 0.0200(7) Uani d S 1 . Na
Na2 0.21797(16) 0.3830(5) 0.70038(11) 0.0170(5) Uani d . 1 . Na
Na3 0.43315(15) 0.3734(5) 0.65425(11) 0.0144(5) Uani d . 1 . Na
Na4 0.65359(16) 0.3746(5) 0.61796(11) 0.0175(5) Uani d . 1 . Na
Na5 0.87129(17) 0.3586(5) 0.57850(11) 0.0191(5) Uani d . 1 . Na
O1 0.1413(3) 0.5918(8) 0.82015(19) 0.0154(8) Uani d . 1 . O
O2 0.3359(3) 0.6214(8) 0.78080(18) 0.0146(8) Uani d . 1 . O
O3 0.4988(3) 0.5845(9) 0.57920(18) 0.0159(9) Uani d . 1 . O
O4 0.0620(3) 0.5919(9) 0.65514(19) 0.0167(9) Uani d . 1 . O
O5 0.7077(3) 0.5817(8) 0.53421(19) 0.0149(8) Uani d . 1 . O
O6 0.2862(3) 0.5847(8) 0.62073(19) 0.0136(8) Uani d . 1 . O
O7 0.9022(3) 0.5698(9) 0.48829(19) 0.0167(9) Uani d . 1 . O
O8 0.5000 0.6910(11) 0.7500 0.0114(11) Uani d S 1 . O
O9 0.7640(2) 0.0423(8) 0.61492(17) 0.0093(7) Uani d . 1 . O
O10 0.5534(2) 0.0486(8) 0.65941(16) 0.0108(8) Uani d . 1 . O
O11 0.3470(2) 0.0485(8) 0.69900(17) 0.0097(7) Uani d . 1 . O
O12 0.1453(3) 0.0323(8) 0.73845(17) 0.0115(8) Uani d . 1 . O
O13 0.0429(2) 0.0421(8) 0.82765(17) 0.0119(7) Uani d . 1 . O
O14 0.1622(2) 0.0356(8) 0.61619(17) 0.0098(7) Uani d . 1 . O
O15 0.3728(2) 0.0330(8) 0.57380(16) 0.0095(7) Uani d . 1 . O
O16 0.5841(2) 0.0388(8) 0.53233(17) 0.0097(7) Uani d . 1 . O
O17 0.7986(2) 0.0301(8) 0.49087(17) 0.0085(7) Uani d . 1 . O
O18 0.9921(2) 0.0323(8) 0.55719(16) 0.0103(8) Uani d . 1 . O
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
O1 V1 O9 . 2_666 111.16(19)
O1 V1 O13 . 1_565 108.4(2)
O9 V1 O13 2_666 1_565 106.92(18)
O1 V1 O12 . 1_565 111.0(2)
O9 V1 O12 2_666 1_565 113.17(18)
O13 V1 O12 1_565 1_565 105.78(18)
O1 V1 Na5 . 2_666 132.38(15)
O9 V1 Na5 2_666 2_666 54.47(13)
O13 V1 Na5 1_565 2_666 53.23(14)
O12 V1 Na5 1_565 2_666 116.18(15)
O1 V1 Na1 . 1_565 136.84(15)
O9 V1 Na1 2_666 1_565 109.45(14)
O13 V1 Na1 1_565 1_565 44.49(13)
O12 V1 Na1 1_565 1_565 63.94(13)
Na5 V1 Na1 2_666 1_565 65.39(6)
O1 V1 Na1 . . 39.08(14)
O9 V1 Na1 2_666 . 147.99(14)
O13 V1 Na1 1_565 . 80.98(14)
O12 V1 Na1 1_565 . 93.40(13)
Na5 V1 Na1 2_666 . 129.69(6)
Na1 V1 Na1 1_565 . 97.89(4)
O1 V1 Na5 . 2_656 36.21(14)
O9 V1 Na5 2_666 2_656 89.63(13)
O13 V1 Na5 1_565 2_656 88.55(14)
O12 V1 Na5 1_565 2_656 147.10(14)
Na5 V1 Na5 2_666 2_656 96.22(6)
Na1 V1 Na5 1_565 2_656 132.22(6)
Na1 V1 Na5 . 2_656 59.12(5)
O2 V2 O11 . 1_565 112.08(18)
O2 V2 O10 . 2_666 110.80(19)
O11 V2 O10 1_565 2_666 111.04(18)
O2 V2 O8 . . 106.7(2)
O11 V2 O8 1_565 . 106.73(15)
O10 V2 O8 2_666 . 109.26(15)
O2 V2 Na3 . 2_656 79.12(15)
O11 V2 Na3 1_565 2_656 149.98(13)
O10 V2 Na3 2_666 2_656 88.79(14)
O8 V2 Na3 . 2_656 43.78(10)
O2 V2 Na3 . . 80.22(15)
O11 V2 Na3 1_565 . 87.62(13)
O10 V2 Na3 2_666 . 150.87(13)
O8 V2 Na3 . . 42.13(10)
Na3 V2 Na3 2_656 . 66.26(7)
O2 V2 Na3 . 2_666 146.21(14)
O11 V2 Na3 1_565 2_666 92.73(14)
O10 V2 Na3 2_666 2_666 36.13(13)
O8 V2 Na3 . 2_666 86.33(14)
Na3 V2 Na3 2_656 2_666 90.80(6)
Na3 V2 Na3 . 2_666 125.09(4)
O2 V2 Na2 . . 30.27(13)
O11 V2 Na2 1_565 . 86.17(14)
O10 V2 Na2 2_666 . 137.97(13)
O8 V2 Na2 . . 101.13(15)
Na3 V2 Na2 2_656 . 93.87(7)
Na3 V2 Na2 . . 62.35(6)
Na3 V2 Na2 2_666 . 172.47(6)
O2 V2 Na3 . 1_565 146.46(13)
O11 V2 Na3 1_565 1_565 35.24(13)
O10 V2 Na3 2_666 1_565 94.01(14)
O8 V2 Na3 . 1_565 84.63(14)
Na3 V2 Na3 2_656 1_565 125.13(4)
Na3 V2 Na3 . 1_565 88.95(5)
Na3 V2 Na3 2_666 1_565 63.78(7)
Na2 V2 Na3 . 1_565 117.57(6)
O3 V3 O16 . 1_565 112.23(18)
O3 V3 O15 . 1_565 111.04(19)
O16 V3 O15 1_565 1_565 136.27(17)
O3 V3 O16 . 3_666 109.51(18)
O16 V3 O16 1_565 3_666 79.75(16)
O15 V3 O16 1_565 3_666 80.36(15)
O3 V3 O10 . 1_565 100.80(17)
O16 V3 O10 1_565 1_565 90.95(15)
O15 V3 O10 1_565 1_565 87.04(15)
O16 V3 O10 3_666 1_565 149.62(17)
O3 V3 V3 . 3_676 117.62(15)
O16 V3 V3 1_565 3_676 40.46(10)
O15 V3 V3 1_565 3_676 110.76(11)
O16 V3 V3 3_666 3_676 39.28(11)
O10 V3 V3 1_565 3_676 125.42(12)
O3 V3 V5 . 3_676 117.68(14)
O16 V3 V5 1_565 3_676 110.17(11)
O15 V3 V5 1_565 3_676 40.50(10)
O16 V3 V5 3_666 3_676 39.88(11)
O10 V3 V5 1_565 3_676 121.92(12)
V3 V3 V5 3_676 3_676 73.48(5)
O3 V3 Na3 . 1_565 129.18(15)
O16 V3 Na3 1_565 1_565 107.20(13)
O15 V3 Na3 1_565 1_565 44.93(12)
O16 V3 Na3 3_666 1_565 107.92(12)
O10 V3 Na3 1_565 1_565 47.28(12)
V3 V3 Na3 3_676 1_565 113.15(6)
V5 V3 Na3 3_676 1_565 74.66(5)
O3 V3 Na4 . 1_565 127.68(14)
O16 V3 Na4 1_565 1_565 44.81(12)
O15 V3 Na4 1_565 1_565 108.84(13)
O16 V3 Na4 3_666 1_565 109.34(12)
O10 V3 Na4 1_565 1_565 49.31(12)
V3 V3 Na4 3_676 1_565 76.23(6)
V5 V3 Na4 3_676 1_565 114.63(6)
Na3 V3 Na4 1_565 1_565 66.56(6)
O3 V3 Na3 . . 34.94(14)
O16 V3 Na3 1_565 . 143.03(12)
O15 V3 Na3 1_565 . 80.10(12)
O16 V3 Na3 3_666 . 120.80(12)
O10 V3 Na3 1_565 . 83.49(12)
V3 V3 Na3 3_676 . 148.40(6)
V5 V3 Na3 3_676 . 103.63(5)
Na3 V3 Na3 1_565 . 95.63(6)
Na4 V3 Na3 1_565 . 129.85(6)
O3 V3 Na4 . . 36.26(14)
O16 V3 Na4 1_565 . 80.67(12)
O15 V3 Na4 1_565 . 142.19(12)
O16 V3 Na4 3_666 . 122.09(12)
O10 V3 Na4 1_565 . 84.10(12)
V3 V3 Na4 3_676 . 104.24(6)
V5 V3 Na4 3_676 . 150.38(5)
Na3 V3 Na4 1_565 . 129.91(6)
Na4 V3 Na4 1_565 . 92.71(7)
Na3 V3 Na4 . . 62.42(6)
O4 V4 O13 . 2_566 106.93(19)
O4 V4 O12 . 1_565 105.39(18)
O13 V4 O12 2_566 1_565 89.84(16)
O4 V4 O14 . 1_565 111.48(18)
O13 V4 O14 2_566 1_565 141.25(18)
O12 V4 O14 1_565 1_565 85.00(15)
O4 V4 O18 . 1_465 110.62(19)
O13 V4 O18 2_566 1_465 84.07(15)
O12 V4 O18 1_565 1_465 143.71(18)
O14 V4 O18 1_565 1_465 77.98(15)
O4 V4 V7 . 3_676 113.90(14)
O13 V4 V7 2_566 3_676 118.18(12)
O12 V4 V7 1_565 3_676 119.53(12)
O14 V4 V7 1_565 3_676 38.95(10)
O18 V4 V7 1_465 3_676 39.31(11)
O4 V4 Na2 . 1_565 136.69(15)
O13 V4 Na2 2_566 1_565 104.48(13)
O12 V4 Na2 1_565 1_565 45.66(12)
O14 V4 Na2 1_565 1_565 47.77(12)
O18 V4 Na2 1_465 1_565 101.54(13)
V7 V4 Na2 3_676 1_565 74.70(5)
O4 V4 Na2 . . 40.34(15)
O13 V4 Na2 2_566 . 136.13(13)
O12 V4 Na2 1_565 . 78.07(13)
O14 V4 Na2 1_565 . 80.13(12)
O18 V4 Na2 1_465 . 128.87(13)
V7 V4 Na2 3_676 . 104.22(5)
Na2 V4 Na2 1_565 . 96.66(7)
O4 V4 Na1 . 1_565 129.86(15)
O13 V4 Na1 2_566 1_565 38.59(11)
O12 V4 Na1 1_565 1_565 56.36(12)
O14 V4 Na1 1_565 1_565 112.34(13)
O18 V4 Na1 1_465 1_565 101.23(12)
V7 V4 Na1 3_676 1_565 115.31(6)
Na2 V4 Na1 1_565 1_565 67.34(6)
Na2 V4 Na1 . 1_565 129.83(5)
O4 V4 Na5 . 1_465 128.56(15)
O13 V4 Na5 2_566 1_465 42.26(12)
O12 V4 Na5 1_565 1_465 112.32(13)
O14 V4 Na5 1_565 1_465 105.57(12)
O18 V4 Na5 1_465 1_465 45.03(12)
V7 V4 Na5 3_676 1_465 75.93(5)
Na2 V4 Na5 1_565 1_465 94.69(7)
Na2 V4 Na5 . 1_465 168.26(6)
Na1 V4 Na5 1_565 1_465 58.07(5)
O4 V4 Na1 . . 40.79(14)
O13 V4 Na1 2_566 . 72.83(13)
O12 V4 Na1 1_565 . 83.59(12)
O14 V4 Na1 1_565 . 143.93(12)
O18 V4 Na1 1_465 . 127.70(12)
V7 V4 Na1 3_676 . 152.66(5)
Na2 V4 Na1 1_565 . 129.16(5)
Na2 V4 Na1 . . 64.06(6)
Na1 V4 Na1 1_565 . 89.08(2)
Na5 V4 Na1 1_465 . 110.43(6)
O5 V5 O16 . 1_565 112.20(19)
O5 V5 O17 . 1_565 110.29(19)
O16 V5 O17 1_565 1_565 136.84(17)
O5 V5 O15 . 3_666 108.23(18)
O16 V5 O15 1_565 3_666 80.00(15)
O17 V5 O15 1_565 3_666 80.06(15)
O5 V5 O9 . 1_565 103.17(18)
O16 V5 O9 1_565 1_565 87.22(15)
O17 V5 O9 1_565 1_565 90.36(15)
O15 V5 O9 3_666 1_565 148.58(17)
O5 V5 V3 . 3_676 116.06(14)
O16 V5 V3 1_565 3_676 40.43(10)
O17 V5 V3 1_565 3_676 111.45(11)
O15 V5 V3 3_666 3_676 39.57(10)
O9 V5 V3 1_565 3_676 122.45(11)
O5 V5 V6 . 3_676 115.74(14)
O16 V5 V6 1_565 3_676 110.46(11)
O17 V5 V6 1_565 3_676 40.88(10)
O15 V5 V6 3_666 3_676 39.18(11)
O9 V5 V6 1_565 3_676 124.67(12)
V3 V5 V6 3_676 3_676 73.78(4)
O5 V5 Na4 . 1_565 130.63(15)
O16 V5 Na4 1_565 1_565 46.56(12)
O17 V5 Na4 1_565 1_565 106.98(13)
O15 V5 Na4 3_666 1_565 109.11(12)
O9 V5 Na4 1_565 1_565 45.31(11)
V3 V5 Na4 3_676 1_565 77.16(5)
V6 V5 Na4 3_676 1_565 113.62(6)
O5 V5 Na5 . 1_565 127.24(15)
O16 V5 Na5 1_565 1_565 109.53(13)
O17 V5 Na5 1_565 1_565 44.77(11)
O15 V5 Na5 3_666 1_565 109.53(12)
O9 V5 Na5 1_565 1_565 48.50(12)
V3 V5 Na5 3_676 1_565 116.58(6)
V6 V5 Na5 3_676 1_565 76.38(5)
Na4 V5 Na5 1_565 1_565 65.96(7)
O5 V5 Na4 . . 36.16(14)
O16 V5 Na4 1_565 . 82.45(12)
O17 V5 Na4 1_565 . 139.73(12)
O15 V5 Na4 3_666 . 124.10(12)
O9 V5 Na4 1_565 . 81.83(12)
V3 V5 Na4 3_676 . 105.92(5)
V6 V5 Na4 3_676 . 149.77(5)
Na4 V5 Na4 1_565 . 95.24(6)
Na5 V5 Na4 1_565 . 126.36(6)
O6 V6 O14 . 1_565 111.47(19)
O6 V6 O15 . 1_565 111.31(18)
O14 V6 O15 1_565 1_565 136.78(17)
O6 V6 O17 . 3_666 110.52(18)
O14 V6 O17 1_565 3_666 79.48(14)
O15 V6 O17 1_565 3_666 80.28(15)
O6 V6 O11 . 1_565 101.22(18)
O14 V6 O11 1_565 1_565 89.28(15)
O15 V6 O11 1_565 1_565 88.33(15)
O17 V6 O11 3_666 1_565 148.26(16)
O6 V6 V7 . 3_676 119.30(14)
O14 V6 V7 1_565 3_676 40.05(10)
O15 V6 V7 1_565 3_676 110.13(11)
O17 V6 V7 3_666 3_676 39.49(11)
O11 V6 V7 1_565 3_676 122.32(12)
O6 V6 V5 . 3_676 117.58(14)
O14 V6 V5 1_565 3_676 111.02(11)
O15 V6 V5 1_565 3_676 40.24(10)
O17 V6 V5 3_666 3_676 40.04(10)
O11 V6 V5 1_565 3_676 122.73(11)
V7 V6 V5 3_676 3_676 73.78(4)
O6 V6 Na3 . 1_565 129.50(15)
O14 V6 Na3 1_565 1_565 107.41(14)
O15 V6 Na3 1_565 1_565 44.96(12)
O17 V6 Na3 3_666 1_565 107.14(12)
O11 V6 Na3 1_565 1_565 48.16(11)
V7 V6 Na3 3_676 1_565 111.19(6)
V5 V6 Na3 3_676 1_565 74.57(5)
O6 V6 Na2 . 1_565 128.50(14)
O14 V6 Na2 1_565 1_565 43.91(12)
O15 V6 Na2 1_565 1_565 108.83(13)
O17 V6 Na2 3_666 1_565 106.84(12)
O11 V6 Na2 1_565 1_565 49.30(12)
V7 V6 Na2 3_676 1_565 73.10(5)
V5 V6 Na2 3_676 1_565 113.87(6)
Na3 V6 Na2 1_565 1_565 66.91(6)
O6 V6 Na3 . . 35.14(14)
O14 V6 Na3 1_565 . 142.30(13)
O15 V6 Na3 1_565 . 80.27(12)
O17 V6 Na3 3_666 . 122.03(12)
O11 V6 Na3 1_565 . 84.43(12)
V7 V6 Na3 3_676 . 150.52(5)
V5 V6 Na3 3_676 . 103.51(5)
Na3 V6 Na3 1_565 . 95.74(7)
Na2 V6 Na3 1_565 . 131.12(6)
O6 V6 Na2 . . 36.82(14)
O14 V6 Na2 1_565 . 79.00(13)
O15 V6 Na2 1_565 . 143.40(12)
O17 V6 Na2 3_666 . 121.93(12)
O11 V6 Na2 1_565 . 84.07(12)
V7 V6 Na2 3_676 . 104.11(5)
V5 V6 Na2 3_676 . 150.30(5)
Na3 V6 Na2 1_565 . 130.69(6)
Na2 V6 Na2 1_565 . 92.95(6)
Na3 V6 Na2 . . 63.41(6)
O7 V7 O18 . 1_565 108.85(19)
O7 V7 O17 . 1_565 106.43(19)
O18 V7 O17 1_565 1_565 95.61(15)
O7 V7 O14 . 3_666 108.16(19)
O18 V7 O14 1_565 3_666 142.12(18)
O17 V7 O14 1_565 3_666 81.41(15)
O7 V7 O18 . 3_766 110.17(19)
O18 V7 O18 1_565 3_766 80.93(16)
O17 V7 O18 1_565 3_766 142.33(18)
O14 V7 O18 3_666 3_766 79.15(15)
O7 V7 V7 . 3_776 116.05(15)
O18 V7 V7 1_565 3_776 41.20(11)
O17 V7 V7 1_565 3_776 126.25(13)
O14 V7 V7 3_666 3_776 112.66(13)
O18 V7 V7 3_766 3_776 39.72(10)
O7 V7 V6 . 3_676 111.53(14)
O18 V7 V6 1_565 3_676 127.63(13)
O17 V7 V6 1_565 3_676 41.69(10)
O14 V7 V6 3_666 3_676 39.77(11)
O18 V7 V6 3_766 3_676 113.56(11)
V7 V7 V6 3_776 3_676 131.44(6)
O7 V7 V4 . 3_676 118.90(14)
O18 V7 V4 1_565 3_676 112.26(12)
O17 V7 V4 1_565 3_676 112.18(11)
O14 V7 V4 3_666 3_676 39.41(11)
O18 V7 V4 3_766 3_676 40.03(10)
V7 V7 V4 3_776 3_676 74.59(5)
V6 V7 V4 3_676 3_676 74.67(4)
O7 V7 Na5 . 1_565 126.75(15)
O18 V7 Na5 1_565 1_565 51.10(13)
O17 V7 Na5 1_565 1_565 46.10(12)
O14 V7 Na5 3_666 1_565 109.53(13)
O18 V7 Na5 3_766 1_565 112.75(13)
V7 V7 Na5 3_776 1_565 81.46(6)
V6 V7 Na5 3_676 1_565 78.00(5)
V4 V7 Na5 3_676 1_565 114.17(6)
O7 V7 Na5 . . 32.33(14)
O18 V7 Na5 1_565 . 88.50(12)
O17 V7 Na5 1_565 . 84.14(12)
O14 V7 Na5 3_666 . 128.25(13)
O18 V7 Na5 3_766 . 132.85(13)
V7 V7 Na5 3_776 . 115.89(6)
V6 V7 Na5 3_676 . 109.21(6)
V4 V7 Na5 3_676 . 151.09(5)
Na5 V7 Na5 1_565 . 94.43(6)
O13 Na1 O13 2_556 . 80.7(2)
O13 Na1 O1 2_556 . 136.27(15)
O13 Na1 O1 . . 84.21(14)
O13 Na1 O1 2_556 2_556 84.21(14)
O13 Na1 O1 . 2_556 136.27(15)
O1 Na1 O1 . 2_556 131.9(2)
O13 Na1 O4 2_556 2_556 134.87(15)
O13 Na1 O4 . 2_556 81.68(13)
O1 Na1 O4 . 2_556 82.16(15)
O1 Na1 O4 2_556 2_556 80.59(14)
O13 Na1 O4 2_556 . 81.68(13)
O13 Na1 O4 . . 134.87(15)
O1 Na1 O4 . . 80.59(14)
O1 Na1 O4 2_556 . 82.16(15)
O4 Na1 O4 2_556 . 136.8(3)
O13 Na1 O12 2_556 2_556 62.02(13)
O13 Na1 O12 . 2_556 60.85(13)
O1 Na1 O12 . 2_556 139.21(13)
O1 Na1 O12 2_556 2_556 75.79(13)
O4 Na1 O12 2_556 2_556 73.08(12)
O4 Na1 O12 . 2_556 138.80(13)
O13 Na1 O12 2_556 . 60.85(13)
O13 Na1 O12 . . 62.02(13)
O1 Na1 O12 . . 75.79(13)
O1 Na1 O12 2_556 . 139.21(13)
O4 Na1 O12 2_556 . 138.80(12)
O4 Na1 O12 . . 73.08(12)
O12 Na1 O12 2_556 . 102.30(19)
O13 Na1 V1 2_556 1_545 74.16(13)
O13 Na1 V1 . 1_545 31.01(9)
O1 Na1 V1 . 1_545 71.93(11)
O1 Na1 V1 2_556 1_545 156.18(15)
O4 Na1 V1 2_556 1_545 107.67(10)
O4 Na1 V1 . 1_545 103.99(11)
O12 Na1 V1 2_556 1_545 85.16(12)
O12 Na1 V1 . 1_545 32.26(8)
O13 Na1 V1 2_556 2_546 31.01(9)
O13 Na1 V1 . 2_546 74.16(13)
O1 Na1 V1 . 2_546 156.18(15)
O1 Na1 V1 2_556 2_546 71.93(11)
O4 Na1 V1 2_556 2_546 103.99(11)
O4 Na1 V1 . 2_546 107.67(10)
O12 Na1 V1 2_556 2_546 32.25(8)
O12 Na1 V1 . 2_546 85.16(12)
V1 Na1 V1 1_545 2_546 84.32(10)
O13 Na1 V1 2_556 2_556 107.75(10)
O13 Na1 V1 . 2_556 149.74(9)
O1 Na1 V1 . 2_556 105.86(15)
O1 Na1 V1 2_556 2_556 26.02(11)
O4 Na1 V1 2_556 2_556 71.85(11)
O4 Na1 V1 . 2_556 75.38(12)
O12 Na1 V1 2_556 2_556 96.70(8)
O12 Na1 V1 . 2_556 147.68(8)
V1 Na1 V1 1_545 2_556 177.79(9)
V1 Na1 V1 2_546 2_556 97.89(4)
O13 Na1 V1 2_556 . 149.74(9)
O13 Na1 V1 . . 107.75(10)
O1 Na1 V1 . . 26.02(11)
O1 Na1 V1 2_556 . 105.86(15)
O4 Na1 V1 2_556 . 75.38(12)
O4 Na1 V1 . . 71.85(11)
O12 Na1 V1 2_556 . 147.68(8)
O12 Na1 V1 . . 96.70(9)
V1 Na1 V1 1_545 . 97.89(4)
V1 Na1 V1 2_546 . 177.79(9)
V1 Na1 V1 2_556 . 79.90(9)
O2 Na2 O12 . . 118.58(15)
O2 Na2 O14 . . 152.97(17)
O12 Na2 O14 . . 66.97(14)
O2 Na2 O6 . . 82.84(15)
O12 Na2 O6 . . 152.84(17)
O14 Na2 O6 . . 86.38(15)
O2 Na2 O4 . . 117.78(18)
O12 Na2 O4 . . 87.18(16)
O14 Na2 O4 . . 88.12(15)
O6 Na2 O4 . . 97.53(15)
O2 Na2 O11 . . 86.34(15)
O12 Na2 O11 . . 87.46(15)
O14 Na2 O11 . . 67.06(13)
O6 Na2 O11 . . 76.88(14)
O4 Na2 O11 . . 154.69(16)
O2 Na2 V4 . 1_545 154.76(13)
O12 Na2 V4 . 1_545 36.26(9)
O14 Na2 V4 . 1_545 36.69(9)
O6 Na2 V4 . 1_545 120.41(12)
O4 Na2 V4 . 1_545 71.79(12)
O11 Na2 V4 . 1_545 89.59(12)
O2 Na2 V6 . 1_545 119.69(13)
O12 Na2 V6 . 1_545 83.94(12)
O14 Na2 V6 . 1_545 33.43(9)
O6 Na2 V6 . 1_545 70.26(11)
O4 Na2 V6 . 1_545 118.52(12)
O11 Na2 V6 . 1_545 36.25(8)
V4 Na2 V6 1_545 1_545 65.86(6)
O2 Na2 V4 . . 96.01(13)
O12 Na2 V4 . . 109.36(13)
O14 Na2 V4 . . 107.12(11)
O6 Na2 V4 . . 82.64(12)
O4 Na2 V4 . . 25.02(11)
O11 Na2 V4 . . 158.94(12)
V4 Na2 V4 1_545 . 96.66(7)
V6 Na2 V4 1_545 . 130.43(7)
O2 Na2 V6 . . 75.37(11)
O12 Na2 V6 . . 165.33(12)
O14 Na2 V6 . . 102.94(11)
O6 Na2 V6 . . 23.38(10)
O4 Na2 V6 . . 81.71(12)
O11 Na2 V6 . . 98.52(11)
V4 Na2 V6 1_545 . 129.87(7)
V6 Na2 V6 1_545 . 92.95(6)
V4 Na2 V6 . . 62.20(5)
O2 Na2 V2 . . 20.60(9)
O12 Na2 V2 . . 139.08(12)
O14 Na2 V2 . . 143.66(12)
O6 Na2 V2 . . 62.78(11)
O4 Na2 V2 . . 113.21(14)
O11 Na2 V2 . . 86.49(11)
V4 Na2 V2 1_545 . 174.19(8)
V6 Na2 V2 1_545 . 112.59(7)
V4 Na2 V2 . . 88.50(7)
V6 Na2 V2 . . 55.13(4)
O2 Na2 Na4 . 2_656 40.54(11)
O12 Na2 Na4 . 2_656 78.12(11)
O14 Na2 Na4 . 2_656 133.08(13)
O6 Na2 Na4 . 2_656 120.34(12)
O4 Na2 Na4 . 2_656 121.35(13)
O11 Na2 Na4 . 2_656 81.53(10)
V4 Na2 Na4 1_545 2_656 114.22(8)
V6 Na2 Na4 1_545 2_656 115.85(8)
V4 Na2 Na4 . 2_656 113.61(8)
V6 Na2 Na4 . 2_656 115.90(7)
V2 Na2 Na4 . 2_656 60.96(6)
O15 Na3 O3 . . 90.54(15)
O15 Na3 O6 . . 90.43(15)
O3 Na3 O6 . . 99.50(16)
O15 Na3 O10 . . 69.79(13)
O3 Na3 O10 . . 81.85(15)
O6 Na3 O10 . . 160.21(17)
O15 Na3 O11 . . 69.71(14)
O3 Na3 O11 . . 160.25(17)
O6 Na3 O11 . . 80.95(15)
O10 Na3 O11 . . 91.20(15)
O15 Na3 O8 . . 173.10(17)
O3 Na3 O8 . . 95.05(15)
O6 Na3 O8 . . 92.62(14)
O10 Na3 O8 . . 106.98(13)
O11 Na3 O8 . . 104.67(13)
O15 Na3 V6 . 1_545 35.34(9)
O3 Na3 V6 . 1_545 123.22(13)
O6 Na3 V6 . 1_545 73.31(12)
O10 Na3 V6 . 1_545 89.34(12)
O11 Na3 V6 . 1_545 37.76(9)
O8 Na3 V6 . 1_545 140.50(10)
O15 Na3 V3 . 1_545 35.45(9)
O3 Na3 V3 . 1_545 73.26(12)
O6 Na3 V3 . 1_545 123.16(12)
O10 Na3 V3 . 1_545 38.11(9)
O11 Na3 V3 . 1_545 89.85(12)
O8 Na3 V3 . 1_545 143.37(10)
V6 Na3 V3 1_545 1_545 66.33(6)
O15 Na3 V2 . 2_656 152.72(12)
O3 Na3 V2 . 2_656 66.14(11)
O6 Na3 V2 . 2_656 106.63(13)
O10 Na3 V2 . 2_656 92.04(12)
O11 Na3 V2 . 2_656 132.92(11)
O8 Na3 V2 . 2_656 30.69(5)
V6 Na3 V2 1_545 2_656 170.64(8)
V3 Na3 V2 1_545 2_656 119.45(7)
O15 Na3 V6 . . 106.14(12)
O3 Na3 V6 . . 82.37(12)
O6 Na3 V6 . . 23.19(10)
O10 Na3 V6 . . 163.65(12)
O11 Na3 V6 . . 102.34(12)
O8 Na3 V6 . . 78.67(11)
V6 Na3 V6 1_545 . 95.74(7)
V3 Na3 V6 1_545 . 131.51(7)
V2 Na3 V6 2_656 . 85.47(7)
O15 Na3 V3 . . 106.15(11)
O3 Na3 V3 . . 23.14(11)
O6 Na3 V3 . . 82.37(12)
O10 Na3 V3 . . 103.19(12)
O11 Na3 V3 . . 162.76(12)
O8 Na3 V3 . . 80.40(11)
V6 Na3 V3 1_545 . 131.53(7)
V3 Na3 V3 1_545 . 95.63(6)
V2 Na3 V3 2_656 . 57.01(5)
V6 Na3 V3 . . 62.03(5)
O15 Na3 V2 . . 150.52(12)
O3 Na3 V2 . . 108.05(13)
O6 Na3 V2 . . 64.58(11)
O10 Na3 V2 . . 134.02(11)
O11 Na3 V2 . . 90.10(11)
O8 Na3 V2 . . 29.66(5)
V6 Na3 V2 1_545 . 117.43(7)
V3 Na3 V2 1_545 . 172.12(8)
V2 Na3 V2 2_656 . 55.86(5)
V6 Na3 V2 . . 56.09(4)
V3 Na3 V2 . . 86.68(6)
O9 Na4 O5 . . 82.82(15)
O9 Na4 O2 . 2_656 122.67(15)
O5 Na4 O2 . 2_656 118.07(18)
O9 Na4 O16 . . 68.51(14)
O5 Na4 O16 . . 86.64(15)
O2 Na4 O16 2_656 . 152.74(17)
O9 Na4 O3 . . 153.86(17)
O5 Na4 O3 . . 95.35(16)
O2 Na4 O3 2_656 . 81.24(15)
O16 Na4 O3 . . 85.36(15)
O9 Na4 O10 . . 93.38(15)
O5 Na4 O10 . . 154.62(16)
O2 Na4 O10 2_656 . 85.10(15)
O16 Na4 O10 . . 68.76(13)
O3 Na4 O10 . . 77.12(15)
O9 Na4 V5 . 1_545 36.20(9)
O5 Na4 V5 . 1_545 72.20(12)
O2 Na4 V5 2_656 1_545 158.04(13)
O16 Na4 V5 . 1_545 35.59(9)
O3 Na4 V5 . 1_545 118.48(12)
O10 Na4 V5 . 1_545 89.93(11)
O9 Na4 V3 . 1_545 87.16(12)
O5 Na4 V3 . 1_545 117.63(13)
O2 Na4 V3 2_656 1_545 118.85(13)
O16 Na4 V3 . 1_545 33.89(9)
O3 Na4 V3 . 1_545 70.51(12)
O10 Na4 V3 . 1_545 36.99(8)
V5 Na4 V3 1_545 1_545 64.61(6)
O9 Na4 V5 . . 104.19(12)
O5 Na4 V5 . . 23.45(10)
O2 Na4 V5 2_656 . 97.76(13)
O16 Na4 V5 . . 103.30(11)
O3 Na4 V5 . . 80.44(12)
O10 Na4 V5 . . 156.68(12)
V5 Na4 V5 1_545 . 95.24(6)
V3 Na4 V5 1_545 . 127.51(7)
O9 Na4 V3 . . 160.43(12)
O5 Na4 V3 . . 79.91(12)
O2 Na4 V3 2_656 . 74.21(12)
O16 Na4 V3 . . 101.19(11)
O3 Na4 V3 . . 22.91(11)
O10 Na4 V3 . . 98.27(12)
V5 Na4 V3 1_545 . 127.72(7)
V3 Na4 V3 1_545 . 92.71(7)
V5 Na4 V3 . . 60.85(5)
O9 Na4 Na2 . 2_656 83.81(11)
O5 Na4 Na2 . 2_656 123.64(13)
O2 Na4 Na2 2_656 2_656 39.31(10)
O16 Na4 Na2 . 2_656 136.43(13)
O3 Na4 Na2 . 2_656 117.75(12)
O10 Na4 Na2 . 2_656 80.53(10)
V5 Na4 Na2 1_545 2_656 118.76(8)
V3 Na4 Na2 1_545 2_656 116.03(8)
V5 Na4 Na2 . 2_656 116.08(8)
V3 Na4 Na2 . 2_656 113.52(8)
O9 Na4 Na5 . . 44.24(11)
O5 Na4 Na5 . . 45.28(11)
O2 Na4 Na5 2_656 . 113.63(13)
O16 Na4 Na5 . . 91.67(11)
O3 Na4 Na5 . . 140.63(13)
O10 Na4 Na5 . . 137.58(14)
V5 Na4 Na5 1_545 . 58.16(6)
V3 Na4 Na5 1_545 . 122.74(9)
V5 Na4 Na5 . . 62.05(6)
V3 Na4 Na5 . . 122.90(8)
Na2 Na4 Na5 2_656 . 90.86(8)
O7 Na5 O17 . . 82.55(15)
O7 Na5 O1 . 2_656 124.03(18)
O17 Na5 O1 . 2_656 144.62(17)
O7 Na5 O13 . 2_656 135.99(16)
O17 Na5 O13 . 2_656 98.15(15)
O1 Na5 O13 2_656 2_656 78.85(14)
O7 Na5 O9 . . 146.60(16)
O17 Na5 O9 . . 67.84(13)
O1 Na5 O9 2_656 . 79.06(14)
O13 Na5 O9 2_656 . 66.30(13)
O7 Na5 O18 . . 79.23(15)
O17 Na5 O18 . . 67.54(13)
O1 Na5 O18 2_656 . 134.33(15)
O13 Na5 O18 2_656 . 61.23(12)
O9 Na5 O18 . . 102.09(15)
O7 Na5 O5 . . 86.50(15)
O17 Na5 O5 . . 83.22(14)
O1 Na5 O5 2_656 . 76.45(14)
O13 Na5 O5 2_656 . 137.46(15)
O9 Na5 O5 . . 75.33(14)
O18 Na5 O5 . . 148.75(15)
O7 Na5 V1 . 2_646 161.73(15)
O17 Na5 V1 . 2_646 85.18(11)
O1 Na5 V1 2_656 2_646 73.02(11)
O13 Na5 V1 2_656 2_646 33.42(9)
O9 Na5 V1 . 2_646 33.26(8)
O18 Na5 V1 . 2_646 83.60(11)
O5 Na5 V1 . 2_646 105.46(12)
O7 Na5 V7 . 1_545 72.94(13)
O17 Na5 V7 . 1_545 34.24(9)
O1 Na5 V7 2_656 1_545 161.44(13)
O13 Na5 V7 2_656 1_545 83.24(11)
O9 Na5 V7 . 1_545 89.38(11)
O18 Na5 V7 . 1_545 34.27(8)
O5 Na5 V7 . 1_545 114.83(12)
V1 Na5 V7 2_646 1_545 89.34(7)
O7 Na5 V5 . 1_545 111.84(13)
O17 Na5 V5 . 1_545 34.42(9)
O1 Na5 V5 2_656 1_545 110.32(13)
O13 Na5 V5 2_656 1_545 88.81(12)
O9 Na5 V5 . 1_545 35.36(8)
O18 Na5 V5 . 1_545 91.16(12)
O5 Na5 V5 . 1_545 68.51(11)
V1 Na5 V5 2_646 1_545 62.06(5)
V7 Na5 V5 1_545 1_545 64.18(6)
O7 Na5 Na1 . 1_655 127.21(15)
O17 Na5 Na1 . 1_655 140.65(14)
O1 Na5 Na1 2_656 1_655 43.17(10)
O13 Na5 Na1 2_656 1_655 42.99(11)
O9 Na5 Na1 . 1_655 86.18(10)
O18 Na5 Na1 . 1_655 91.16(11)
O5 Na5 Na1 . 1_655 119.34(12)
V1 Na5 Na1 2_646 1_655 58.92(7)
V7 Na5 Na1 1_545 1_655 122.29(9)
V5 Na5 Na1 1_545 1_655 120.22(9)
O7 Na5 V7 . . 21.49(11)
O17 Na5 V7 . . 100.68(11)
O1 Na5 V7 2_656 . 102.69(13)
O13 Na5 V7 2_656 . 142.27(12)
O9 Na5 V7 . . 151.42(12)
O18 Na5 V7 . . 96.77(11)
O5 Na5 V7 . . 77.39(11)
V1 Na5 V7 2_646 . 173.83(8)
V7 Na5 V7 1_545 . 94.43(6)
V5 Na5 V7 1_545 . 124.04(7)
Na1 Na5 V7 1_655 . 114.91(9)
V1 O1 Na1 . . 114.9(2)
V1 O1 Na5 . 2_656 120.6(2)
Na1 O1 Na5 . 2_656 91.33(15)
V2 O2 Na2 . . 129.1(2)
V2 O2 Na4 . 2_656 130.0(2)
Na2 O2 Na4 . 2_656 100.15(17)
V3 O3 Na3 . . 121.9(2)
V3 O3 Na4 . . 120.8(2)
Na3 O3 Na4 . . 98.93(16)
V4 O4 Na2 . . 114.6(2)
V4 O4 Na1 . . 115.5(2)
Na2 O4 Na1 . . 95.26(15)
V5 O5 Na4 . . 120.4(2)
V5 O5 Na5 . . 120.2(2)
Na4 O5 Na5 . . 94.01(15)
V6 O6 Na3 . . 121.7(2)
V6 O6 Na2 . . 119.8(2)
Na3 O6 Na2 . . 100.50(16)
V7 O7 Na5 . . 126.2(2)
V2 O8 V2 2_656 . 126.2(3)
V2 O8 Na3 2_656 2_656 108.20(9)
V2 O8 Na3 . 2_656 105.53(8)
V2 O8 Na3 2_656 . 105.53(8)
V2 O8 Na3 . . 108.20(8)
Na3 O8 Na3 2_656 . 100.3(2)
V1 O9 V5 2_646 1_545 131.6(2)
V1 O9 Na4 2_646 . 128.10(19)
V5 O9 Na4 1_545 . 98.49(15)
V1 O9 Na5 2_646 . 92.28(16)
V5 O9 Na5 1_545 . 96.14(14)
Na4 O9 Na5 . . 95.30(16)
V2 O10 V3 2_646 1_545 124.3(2)
V2 O10 Na3 2_646 . 119.16(18)
V3 O10 Na3 1_545 . 94.61(15)
V2 O10 Na4 2_646 . 123.25(18)
V3 O10 Na4 1_545 . 93.70(14)
Na3 O10 Na4 . . 94.26(16)
V2 O11 V6 1_545 1_545 124.1(2)
V2 O11 Na3 1_545 . 121.00(18)
V6 O11 Na3 1_545 . 94.08(14)
V2 O11 Na2 1_545 . 121.67(18)
V6 O11 Na2 1_545 . 94.45(14)
Na3 O11 Na2 . . 94.00(15)
V1 O12 V4 1_545 1_545 126.2(2)
V1 O12 Na2 1_545 . 135.2(2)
V4 O12 Na2 1_545 . 98.08(15)
V1 O12 Na1 1_545 . 83.81(14)
V4 O12 Na1 1_545 . 90.33(14)
Na2 O12 Na1 . . 90.14(15)
V1 O13 V4 1_545 2_546 138.8(2)
V1 O13 Na1 1_545 . 104.50(17)
V4 O13 Na1 2_546 . 110.76(16)
V1 O13 Na5 1_545 2_656 93.36(16)
V4 O13 Na5 2_546 2_656 106.80(16)
Na1 O13 Na5 . 2_656 90.21(16)
V6 O14 V7 1_545 3_666 100.18(16)
V6 O14 V4 1_545 1_545 138.3(2)
V7 O14 V4 3_666 1_545 101.64(16)
V6 O14 Na2 1_545 . 102.66(16)
V7 O14 Na2 3_666 . 121.5(2)
V4 O14 Na2 1_545 . 95.54(15)
V6 O15 V3 1_545 1_545 137.2(2)
V6 O15 V5 1_545 3_666 100.58(16)
V3 O15 V5 1_545 3_666 99.92(15)
V6 O15 Na3 1_545 . 99.70(15)
V3 O15 Na3 1_545 . 99.62(16)
V5 O15 Na3 3_666 . 123.42(19)
V3 O16 V5 1_545 1_545 135.3(2)
V3 O16 V3 1_545 3_666 100.25(16)
V5 O16 V3 1_545 3_666 99.69(16)
V3 O16 Na4 1_545 . 101.30(15)
V5 O16 Na4 1_545 . 97.85(15)
V3 O16 Na4 3_666 . 126.99(19)
V7 O17 V5 1_545 1_545 136.0(2)
V7 O17 V6 1_545 3_666 98.83(16)
V5 O17 V6 1_545 3_666 99.07(16)
V7 O17 Na5 1_545 . 99.66(16)
V5 O17 Na5 1_545 . 100.81(15)
V6 O17 Na5 3_666 . 127.18(19)
V7 O18 V7 1_545 3_766 99.07(16)
V7 O18 V4 1_545 1_645 137.2(2)
V7 O18 V4 3_766 1_645 100.66(16)
V7 O18 Na5 1_545 . 94.63(15)
V7 O18 Na5 3_766 . 127.5(2)
V4 O18 Na5 1_645 . 102.57(15)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
V1 O1 . 1.649(4) yes
V1 O9 2_666 1.727(4) yes
V1 O13 1_565 1.736(4) yes
V1 O12 1_565 1.751(4) yes
V1 Na5 2_666 3.146(3) ?
V1 Na1 1_565 3.262(3) ?
V1 Na1 . 3.410(3) ?
V1 Na5 2_656 3.601(3) ?
V2 O2 . 1.634(4) yes
V2 O11 1_565 1.716(4) yes
V2 O10 2_666 1.720(4) yes
V2 O8 . 1.840(3) yes
V2 Na3 2_656 3.472(3) ?
V2 Na3 . 3.531(2) ?
V2 Na3 2_666 3.594(3) ?
V2 Na2 . 3.601(3) ?
V2 Na3 1_565 3.651(3) ?
V3 O3 . 1.619(5) yes
V3 O16 1_565 1.922(4) yes
V3 O15 1_565 1.937(4) yes
V3 O16 3_666 1.970(3) yes
V3 O10 1_565 2.038(4) yes
V3 V3 3_676 2.9876(17) ?
V3 V5 3_676 2.9947(19) ?
V3 Na3 1_565 3.292(3) ?
V3 Na4 1_565 3.381(3) ?
V3 Na3 . 3.496(3) ?
V3 Na4 . 3.571(3) ?
V4 O4 . 1.619(5) yes
V4 O13 2_566 1.930(4) yes
V4 O12 1_565 1.944(4) yes
V4 O14 1_565 1.953(4) yes
V4 O18 1_465 1.972(3) yes
V4 V7 3_676 3.0137(13) ?
V4 Na2 1_565 3.254(3) ?
V4 Na2 . 3.479(3) ?
V4 Na1 1_565 3.540(3) ?
V4 Na5 1_465 3.594(3) ?
V4 Na1 . 3.633(3) ?
V5 O5 . 1.612(4) yes
V5 O16 1_565 1.948(4) yes
V5 O17 1_565 1.957(4) yes
V5 O15 3_666 1.975(3) yes
V5 O9 1_565 1.980(3) yes
V5 V3 3_676 2.9948(19) ?
V5 V6 3_676 3.0044(13) ?
V5 Na4 1_565 3.315(3) ?
V5 Na5 1_565 3.401(3) ?
V5 Na4 . 3.495(3) ?
V6 O6 . 1.616(4) yes
V6 O14 1_565 1.923(4) yes
V6 O15 1_565 1.931(4) yes
V6 O17 3_666 1.991(3) yes
V6 O11 1_565 2.020(4) yes
V6 V7 3_676 2.9589(19) ?
V6 V5 3_676 3.0044(13) ?
V6 Na3 1_565 3.290(3) ?
V6 Na2 1_565 3.406(3) ?
V6 Na3 . 3.492(3) ?
V6 Na2 . 3.533(3) ?
V7 O7 . 1.597(5) yes
V7 O18 1_565 1.885(4) yes
V7 O17 1_565 1.904(4) yes
V7 O14 3_666 1.934(3) yes
V7 O18 3_766 1.943(4) yes
V7 V7 3_776 2.912(2) ?
V7 V6 3_676 2.9589(19) ?
V7 V4 3_676 3.0138(13) ?
V7 Na5 1_565 3.336(3) ?
V7 Na5 . 3.518(3) ?
Na1 O13 2_556 2.361(5) yes
Na1 O13 . 2.361(5) yes
Na1 O1 . 2.370(4) yes
Na1 O1 2_556 2.370(4) yes
Na1 O4 2_556 2.629(4) yes
Na1 O4 . 2.629(4) yes
Na1 O12 2_556 2.947(5) yes
Na1 O12 . 2.947(5) yes
Na1 V1 1_545 3.262(3) ?
Na1 V1 2_546 3.262(3) ?
Na1 V1 2_556 3.410(3) ?
Na2 O2 . 2.340(4) yes
Na2 O12 . 2.351(5) yes
Na2 O14 . 2.421(4) yes
Na2 O6 . 2.440(4) yes
Na2 O4 . 2.477(5) yes
Na2 O11 . 2.590(5) yes
Na2 V4 1_545 3.254(3) ?
Na2 V6 1_545 3.406(3) ?
Na2 Na4 2_656 3.636(3) ?
Na3 O15 . 2.358(4) yes
Na3 O3 . 2.359(5) yes
Na3 O6 . 2.362(5) yes
Na3 O10 . 2.427(5) yes
Na3 O11 . 2.457(4) yes
Na3 O8 . 2.493(4) yes
Na3 V6 1_545 3.290(3) ?
Na3 V3 1_545 3.292(3) ?
Na3 V2 2_656 3.472(3) ?
Na4 O9 . 2.383(4) yes
Na4 O5 . 2.391(5) yes
Na4 O2 2_656 2.401(4) yes
Na4 O16 . 2.430(4) yes
Na4 O3 . 2.459(5) yes
Na4 O10 . 2.569(5) yes
Na4 V5 1_545 3.315(3) ?
Na4 V3 1_545 3.381(3) ?
Na4 Na2 2_656 3.636(3) ?
Na4 Na5 . 3.656(4) ?
Na5 O7 . 2.331(4) yes
Na5 O17 . 2.439(4) yes
Na5 O1 2_656 2.470(5) yes
Na5 O13 2_656 2.524(4) yes
Na5 O9 . 2.562(5) yes
Na5 O18 . 2.605(5) yes
Na5 O5 . 2.604(5) yes
Na5 O4 1_655 3.0470(10) yes
Na5 V1 2_646 3.146(3) ?
Na5 V7 1_545 3.336(3) ?
Na5 V5 1_545 3.401(3) ?
Na5 Na1 1_655 3.463(3) ?
O1 Na5 2_656 2.470(5) ?
O2 Na4 2_656 2.401(4) ?
O8 V2 2_656 1.839(3) ?
O8 Na3 2_656 2.493(4) ?
O9 V1 2_646 1.727(3) ?
O9 V5 1_545 1.980(3) ?
O10 V2 2_646 1.720(4) ?
O10 V3 1_545 2.038(3) ?
O11 V2 1_545 1.716(4) ?
O11 V6 1_545 2.020(4) ?
O12 V1 1_545 1.751(4) ?
O12 V4 1_545 1.944(4) ?
O13 V1 1_545 1.736(4) ?
O13 V4 2_546 1.930(4) ?
O13 Na5 2_656 2.524(4) ?
O14 V6 1_545 1.923(4) ?
O14 V7 3_666 1.934(3) ?
O14 V4 1_545 1.954(4) ?
O15 V6 1_545 1.931(4) ?
O15 V3 1_545 1.937(4) ?
O15 V5 3_666 1.974(3) ?
O16 V3 1_545 1.922(4) ?
O16 V5 1_545 1.948(4) ?
O16 V3 3_666 1.970(3) ?
O17 V7 1_545 1.904(4) ?
O17 V5 1_545 1.957(4) ?
O17 V6 3_666 1.991(3) ?
O18 V7 1_545 1.885(4) ?
O18 V7 3_766 1.943(4) ?
O18 V4 1_645 1.972(3) ?
